Preparative methods of cellulose/metal nanocomposites.
Research on inorganic/organic nanocomposite materials is a fast growing interdisciplinary area in materials science and engineering. In particular, extensive work has been undertaken in the development of sustainable and environmentally friendly resources and methods. A key idea has been the production of nanocomposites comprising biopolymers that in specific contexts can replace conventional materials such as synthetic polymers. It is well known that the properties of nanocomposite materials depend not only on the properties of their individual components but also on morphological and interfacial characteristics arising from the combination of distinct materials . Therefore the use of polymers such as cellulose, starch, alginate, dextran, carrageenan, and chitosan among others, gain great relevance not only due to their renewable nature and biodegradability, but also because a variety of formulations can be exploited depending on the envisaged functionality [2, 3].
This chapter has focus on the use of cellulose as the matrix in the production of nanocomposites. Cellulose has critical importance namely because is the most abundant and widespread biopolymer on Earth. Owing to its abundance and specific properties, it is important noted for the development of environmental friendly, biocompatible, and functional composites, quite apart from its traditional and massive use in papermaking and cotton textiles . Additionally different types of cellulose are available for the preparation of nanocomposites, namely vegetable cellulose (VC), bacterial cellulose (BC) and nanofibrillated cellulose (NFC). Although sharing similar chemistry and molecular structure, the different kinds of cellulose show important differences in terms of morphology and mechanical behavior. For example, BC and NFC are composed of fibers with nanosized dimensions as compared to VC, which might impart new properties, and in some cases improvements to the ensuing nanocomposite materials .
The association of cellulose with different fillers can bring benefits like improvement of properties (optical, mechanical, …) and delivering unique functions by their use . Cellulose has been used as a soft matrix to accommodate inorganic fillers to produce composites that bring together the intrinsic functionalities of the fillers and the biointerfaces offered by cellulose fibers . Among the wide range of available inorganic fillers, in this review metal nanoparticles (Au, Ag, and Cu, among others) will be considered. Metal NPs exhibit properties that differ from the bulk analogues due to size and surface effects, thus the properties of the final materials can be adjusted as a function of the size, shape, particle size distribution of the nanofillers as well as by interactions occurring with the cellulose fibers’ surfaces. Preparative strategies play a determinant role in the performance and properties of the nanocomposites, hence chemical approaches for the synthesis of these materials are reviewed namely for
2. General aspects on the chemistry and properties of cellulose
The last years have seen great interest in research and application of cellulose nanocomposites namely due to the technological interest in renewable materials and environmentally friendly and sustainable resources . In fact, within the polymers obtained from renewable sources, cellulose is the most abundant natural polymer in Nature as well as the most important component of the plants’"skeleton". This biopolymer formed by repeated connection of glucose building blocks is the structural basis of cell walls of virtually all plants and is usually considered an almost inexhaustible source of raw materials [8, 9]. Cellulose has particular significance owing its unique structure and distinct tendency to form intra- and inter-molecular bonding. These characteristics influence the cellulose supramolecul ararrangement that together with other practical aspects such as the product origin and processing treatment, have important consequences on the final properties of cellulose. This polymer is the main constituent of softwood and hardwood, representing about 40-45% of dry wood, with wood pulp remaining the most important source for cellulose processing namely in paper fabrication [8, 10, 11]. Wood pulp is also the main industrial feedstock for the production of cellulose regenerate fibers and films. This biopolymer is also used in the synthesis of different cellulose derivatives such as esters and ethers. These derivatives are well-kwon active components in applications which include coatings, pharmaceutics and cosmetics, among others  and also used in numerous hybrids containing metal and metal oxides NPs.
Besides extraction from plants, cellulose can be produced by alternative methods, namely by using different types of microorganisms (certain bacteria, algae or fungi). Among the cellulose-forming bacteria,
Due to the complex and expensive process to produce BC, there has been interest to find other ways to obtain cellulose fibers of nanometric dimensions, namely at an industrial scale . NFC can be obtained from VC fibers by distinct methods including chemical treatment and mechanical disintegration procedures, in the form of aqueous suspensions of nanoscale fibers, leading to high aspect ratio materials (5-30 nm diameter and lengths in micrometer range) with remarkable strength and flexibility [16, 17]. The mechanical properties of NFC make this polymer a good candidate for reinforcement materials in nanocomposites. However, besides their interesting mechanical properties, NFC shows other properties of practical interest. For example, NFC has a large surface area which makes it a promising candidate for filtering membranes. Appropriate chemical modifications performed on NFC result in a versatile additive for paints, lacquers or latex. Due to its biocompatibility, NFC might also be used in food and medical applications [11, 17]. As will be clear in the next section, the properties of the cellulose nanocomposites depend not only on the NPs employed as fillers but also on the type of cellulose matrix used.
From all the cellulose derivatives commonly use on the chemistry market, esters and ethers are the predominant. Although produced since the middle of the eighteen century the actually research is related with their manufacture technological improvement. The mail goal is related with the development of greener processes being investigated the use of ionic liquids (IL), microwaves irradiation and solvent-free systems in the synthesis of this cellulose derivatives. This strategy has been followed for the cellulose derivatives used in specifics applications, such as biomedical and optoelectronic and produced in small amounts. The industries responsible for the production of high amounts of these derivatives (as cellulose acetate) have neglected this mandatory necessity .
3. Cellulose/metal nanocomposites
3.1. Preparative strategies of cellulose/metal nanocomposites
A key aspect to consider in combining metal NPs with cellulose fibers is the methodology to be employed namely by taking in consideration the envisaged applications. In order to exploit the properties of nanocomposites, the NPs should be well dispersed over the matrix without the formation of large aggregates that may compromise the final properties and should as much as possible exhibit a small narrow size distribution. There is critical need to find effective techniques that allow the large-scale production that at the same time maintain control of the NPs dispersion in the cellulose matrix. A number of approaches have been developed to attach metal NPs onto cellulose fibers. Table 1 gives examples of methods employed in the preparation of cellulose/metal nanocomposites.
3.1.1. Blending of components
The blending of inorganic NPs and polymers by promoting their homogeneous mixture to form nanocomposites materials has been widely employed . Although this method offers the advantage of simplicity, the use of cellulose as matrix commonly lead to NPs aggregates that decrease the benefits associated to the presence of nanosized fillers. This process often leads to poor laundering durability of the materials and, for example when Ag NPs have been used, the antibacterial efficiency are lower than expected and discontinuous in time . The direct deposition of Ag and Au NPs, by dropwise addition of the respective colloids onto filter papers, has been reported [21, 22]. Usually, this methodology does not lead to an homogeneous distribution of NPs on the paper substrates and the formation of aggregates at the edge of the droplets during the drying process is common .
In situ reduction of metal salts
The preparation of cellulose/metal nanocomposites by the
||Blending of components||Ag [20, 21], Au |
|Cellulose reducing groups||Ag [24-29], Au [29, 30], Cu [31, 32], Pt [33, 34]|
|External reducing agents||Ag [20, 27, 28, 35-38], Au [27, 36, 39, 40], Cu [31, 41, 42], Pt [27, 36, 43, 44], Co , Pd [27, 36]|
|UV reduction||Ag [28, 46, 47]|
|Electrostatic assembly||Ag [28, 36], Au [36, 39], Cu , Pt , Pd |
|Microwave-assisted preparation||Ag [49-51]|
|Surface pre-modification||Ag , Au [52-54]|
||Cellulose reducing groups||Ag |
|Reducing agents||Ag [19, 28, 37, 43, 56-60], Au [39, 43, 61-63], Cu , Pt [43, 65], Co |
|Electrostatic assembly||Au |
|UV reduction||Ag |
|Surface pre-modification||Ag |
||Blending of components||Ag |
|Electrostatic assembly||Ag |
188.8.131.52. Addition of reducing agents
The most commonly used
The use of hydrazine, hydroxylamine and ascorbic acid together with gelatin or polyvinylpyrrolidone (PVP) as colloidal stabilizers has been investigated . Ascorbic acid acted as an efficient reductant for Ag+ and gelatin a good colloidal stabilizer toavoid NPs coalescence and to control particle size.
Reduction of gold salts by flowing H2 over the cellulose matrix has been reported . This methodology allows the preparation of NPs about 2 nm mean diameter. A facile one-step method, in aqueous medium, makes use of poly (ethyleneimine) (PEI) as reducing and macromolecular linker . In this case the thickness of the Au coating surrounding the cellulose fibers can be adjusted by adding different halides (Fig. 2).
184.108.40.206. Reduction of metals salts by cellulose reducing groups
An alternative route for the
This methodology constitutes a green approach to the synthesis of a variety of metal NPs in cellulose matrices in which no additional reducing agents or colloidal stabilizers are used. Kunitake et al.  have reported pioneer research using VC fibers with following work reporting the use of BC fibers for the production of silver and gold nanostructures [28, 39]. This strategy has been reported for other types of biomaterials, hence Ag NPs have been prepared by using the
In the context of composite science, ionic liquids have attracted substantial interest because of their ability to dissolve biopolymers like cellulose. This has been illustrated in the formation of cellulose/Au nanocomposites . The combined use of cellulose and IL allowed the NPs morphology controlin a process in which the IL was retrieved after metal reduction.The use of unbleached kraft fibers have the advantage of limiting metal leaching due chemical affinity between the NPs and the substrate. In this case NPs are formed directly on the VC fiber surfaces by a redox reaction with the associated lignin. This has not been observed for fibers that do not contain lignin .
220.127.116.11. Photo-induced metal growth using irradiation
3.1.3. Electrostatic assembly
The electrostatic assembly of NPs is based on the sequential adsorption of oppositely charged species on a solid substrate which very often is mediated by ionizable polymers . This assembly technique offers some advantages over other methodologies due to the possibility of a better control of inorganic content in the final nanocomposites, full control of NPs size and morphology, and normally leads to less agglomeration of previously prepared NPs.
Cellulose fibers dispersed in water are negatively charged over a wide pH range (2-10), due to the presence of ionizable moieties such as carboxyl and hydroxyl groups, resulting from chemical processing or from minor polysaccharides such as glucuronoxylans . The deposition of Au NPs [39, 72] onto cellulosic fibers was achieved by previous treatment of fibers using multi-layers of poly (diallyldimethylammonium chloride) (polyDADMAC), poly (sodium 4-styrenesulfonate) (PSS), and again polyDADMAC. The use of a positively charged polyelectrolyte as the outer layer favored electrostatic interactions of the fibers with negatively surface charged Au NPs. This methodology has been also applied to the fabrication of Ag/NFC composites using distinct polyelectrolytes as macromolecular linkers . Another example of an electrostatic assembly procedure was based on the chemical modification of cellulose with (2,3-epoxypropyl) trimethylammonium chloride (EPTAC) [36, 73]. This methodology allowed the grafting of the cellulose substrates with positive ammonium ions which is particularly useful for attachment of metal NPs with surface negatives charge.
3.1.4. Other methodologies
Chemical modification of cellulose can be performed to produce distinct types of cellulose/metal nanocomposites. In this context, common cellulose derivatives such as carboximetilcellulose, cellulose acetate and hydroxypropil cellulose have been used [74-76]. 2,2,6,6-tetramethylpyperidine-1-oxy radical (TEMPO) has been used to oxidize selectively the C6 primary hydroxyl groups of cellulose resulting in the corresponding polyuronic acids . In this context, BC acts as an efficient template with the surface carboxylate groups used to quantitatively anchor metal ions via an ion-exchange reaction. The subsequent reduction of the cationsat the nanofibers’ surfaces originated metal NPs with a narrow size distribution. Chemical surface modification of hydroxyl groups into aminic groups, which act as selective coordination sites  and the use of thiol labeled cellulose through spontaneous chemisorption  has been demonstrated. In the latter, chemical attachment of the NPs onto the fibers’ surface limits particle desorption, hence extending the lifetime of the resulting hybrid materials.
The fabrication of size-controlled metal nanowires using cellulose nanocrystals as biomolecular templates has been reported . This method allowed designing Au nanowires of variable sizes that exhibit unique optical properties by controlling the thicknesses of gold shells. In another approach microwave irradiation was used as an efficient method to prepare cellulose/metal nanocomposites . In this study cellulose was treated in a lithium chloride (LiCl)/ N,N-dimethylacetamide (DMAc) and ascorbic acid mixture to produce a homogeneous distribution of Ag NPs within the cellulose matrix. More recently the same group has reported the use of ethylene glycol as solvent, reducing reagent, and microwave absorber, thus excluding an additional reducing agent . This one-step simultaneous formation of Ag NPs and precipitation of the cellulose is a suitable method due to its characteristics of rapid volumetric heating, high reaction rate, short reaction time, enhanced reaction selectivity, and energy saving [49, 77]. A similar methodology was applied in a one-pot process to produce Ag–cellulose nanocomposites, however in this case the cellulose matrix was used as the reducing and stabilizer agent in water suspensions .
3.2. Metal nanoparticles as cellulosic composite fillers and their applications
There are a variety of metal NPs that can be used as dispersed phases in bionanocomposites with cellulose. In the last decades there has been great progress in the colloidal synthesis of inorganic NPs. Colloidal metal NPs have received great attention due to their unique optical, electronic, magnetic, antimicrobial properties. Their small size, large specific surface area and tunable physico-chemical properties that differ significantly from the bulk analogues led to intense research on their use in composite materials . This section gives examples of research on metal NPs used as fillers in cellulose nanocomposites. The applications of these materials are related with the type of NPs present though new properties arise due to the combined use of the metal NPs and cellulose. Table 2 summarizes important applications of cellulose/metal nanocomposites and a brief description will follow in this section.
Nowadays a renewed interest in Ag antimicrobial materials has reappeared mainly due to the increase of multi-drug resistance of microbial strains to conventional antibiotics. The design of protective medical clothing or antibacterial packaging materials are examples of this current trend . Ag NPs are well known by their strong cytotoxicity towards a broad range of microorganisms, such as bacteria and fungi .
Similarly to other applications, well dispersed Ag NPs in the cellulose matrix are required otherwise the antimicrobial effect decreases. However, important parameters such as particle size distribution, metal content, cationic silver release and interaction with the surface of cellulose are also relevant parameters that influence the antimicrobial activity of these nanocomposites [23, 69]. Due to the high water holding capacity and biocompatibility, BC wound dressing materials with improved antimicrobial activity have been prepared using Ag [57, 60]. Other examples include the development of antibacterial food-packaging materials [35, 80], bactericidal paper for water treatment  and the study of laundering properties of nanocomposites [24, 81].
The cellulose fibers can be chemically functionalized creating reactive sites in order to control the
Nanostructured metals such Ag and Au are well known substrates for surface enhanced Raman scattering (SERS). Strong enhancement of the Raman signals is observed for certain molecules chemisorbed to the surface of these metals. Therefore the combined use of these metal NPs and cellulose is of great interest to develop molecular detection and biosensing platforms . In this context, the use of cellulose nanocomposites might bring several advantages such as the fabrication of handy and low cost substrates in the form of paper products. A study on the use of distinct cellulosic matrices containing Ag NPs has shown that the BC/Ag nanocomposites were more sensitive as compared to the vegetable analogues, namely in biodetection of amino acids . The use of filter paper with Ag NPs or Au NPs demonstrate the potential of these materials as SERS platforms to study diverse analytes such as
A simple and low-cost approach to the fabrication of fuel cells has been described based on a nanostructured Ag electrocatalyst and cellulose. Heat removal of the template and combination with graphite improved oxygen reduction in basic medium .
|Water treatment||Electronic devices|
|Wound dressing||Medical (Drug and protein delivery)|
|Catalytic||Smart papers and textiles|
|Fuel cells||Microfluidics devices|
The noble metal gold has long been a cornerstone precious metal occupying a premier position in the world economy, representing wealth and high value. Traditionally it has been used in its yellow lustrous bulk metallic form for monetary and jewelry applications and over recent decades as an electrical conductor and chemically inert contact material in the electronics industry . Au NPs are among the most studied particles in modern materials science namely due to the number of available methods to produce colloids with uniformparticle sizes and well-defined morphologies. Stable Au NPs colloids have been prepared whose particles surfaces are efficiently stabilized by citrate anions in hydrosols or by alkanethiols when organic solvents are used .
Cellulose/Au nanocomposites have been used as catalysts in glucose oxidation . It has been reported that good dispersion of Au NPs in cellulose allowed effective contact with reactants making these materials good catalysts for the reduction of 4-nitrophenol.  Furthermore, cellulose can be used in several solvents having potential applicability in a variety of reactions. Another interesting possibility is the transformation of renewable biomass resources into valuable chemicals. Selective conversion of cellulose or cellobiose into gluconic acid catalyzed by polyoxometalate-  or CNT-supported by Au NPs  has been demonstrated. Agglomeration of the Au NPs in the cellulose nanocomposites has been described as a major limitation decreasing the catalytic activity of the composite materials.
Cellulose based sensors have great interest in several applications including in fields as diverse as medical diagnosis, environmental control and food safety. It is important to develop materials that show good electron transfer capability, biocompatibility, stability and easy accessibility towards the analyte. Additionally large surface area for immobilization of the analytes, rapid response, high sensitivity, good reproducibility and anti-interference are also required characteristics. As expected, it is a great challenge to develop a single material that include all these important characteristics .
Cellulose based sensors are inexpensive, disposable, and environmentally friendly. These materials transport liquids via capillary action with no need of external power . BC/Au nanocomposites have been reported to exhibit good sensitivity, low detection limit and fast response toward hydrogen peroxide makingthese materials suitable matrices for enzyme immobilization [61-63]. The practical application of these nanocomposites for glucose biosensors in human blood samples has been reported. The values obtained showed good agreement with corresponding values obtained in hospital trials. The entrapment of Au NPs and enzymes in a paper coating material of sol–gel derived silica has been reported as a versatile material to be used as an entrapment medium and hydrophobic agent. This characteristic allowed more reproducible enzyme loading on rough and non-uniform paper surfaces .
Conductive or semi-conductive nanocomposites containing Au NPs are very attractive for electronic applications. Although uniform NPs dispersions are required for many applications, for some cases controlled aggregation isused as an advantage. Electrical conductive cellulose films containing Au NPs have been prepared by self-assembly showing electrically conducting above a gold loading of 20 wt % . The mechanism of electronic conduction in Au NPs-cellulose films is strongly dependent on the resistivity of the film .
Copper NPs were found to be good candidates as efficient catalysts in hydrogen production . An important use for Cu NPs include the fabrication of low electrical resistance materials due to their remarkable conductive properties . In addition Cu NPs and their oxides show broad spectrum biocide effects and the antimicrobial activity has been reported in studies of growth inhibition of bacteria, fungus, and algae .
Antimicrobial nanocoatings of Cu NPs on cellulose have been fabricated via electrostatic assembly . In this process, a chemical pre-treatment step was performed in order to impart surface charge on the cotton substrate that promoted binding of cupric ions, followed by chemical reduction to yield metal nanostructured coatings. The resulting composites showed high effectiveness killing to multi-drug resistant pathogen
The use of microcrystalline cellulose as a porous natural material supporting copper ions has been demonstrated [31, 42]. Reducing agent and respective amount have critical importance to achieve Cu NPs (or the metal oxides) with controlled particle size. Conversion of CuO into Cu using cellulose as a reducing agent under alkaline hydrothermal conditions was described as a green process for the production of Cu at power low cost . This process gives rise to the conversion of cellulose into value-added chemicals, such as lactic acid and acetic acid. The possibility of modifying the surface of cellulosic fibers and using chitosan has also been reported . In this case, chitosan-attached cellulose fibers were used in the immobilization of Cu ions followed by a reduction step in the presence of borohydride to obtain Cu NPs. Unlike Au e Ag, non-coated Cu NPs oxidize extensively under ambient atmosphere. Although this detrimental effect is limited by incorporating the Cu NPs in bacterial cellulose, stable Cu/cellulose composites have been prepared by using Cu nanowires as inorganic fillers . These nanocomposites are attractive for the emerging technologies based on electronic paper.
Platinum is an useful material for numerous industrial catalytic applications and several reports have described the synthesis of Pt NPs using a variety of methods . This metal is also considered the best electrocatalyst for the four-electron reduction of oxygen to water in acidic environments as it provides the lowest overpotential and the highest stability . The preparation of Pt/cellulose nanocomposites generally involves the reduction of ionic Pt by addition of a reducing agent (NaBH4, HCHO, …) in the presence of cellulose, which might act as a structural-directing agent .
Nanocomposites of Pt and amorphous carbon films were obtained by the catalyzed carbonization of cellulose fibers . This type of NPs has been synthesized using NaBH4 as reducing agent in hydrothermal conditions in the presence of nanoporous cellulose . The Pt NPs were well dispersed and stabilized in the cellulose network thus avoiding particle aggregation. Cationic cellulose bearing ammonium ions at the surface has also been used to produce this type of nanocomposites . In this method, the attachment of negatively charged Pt NPs onto cationic cellulose substrates was promoted via electrostatic interactions, which result into high surface coverage of the fibers.
Thermally stable proton-conducting membranes have been prepared by the
The incorporation of irregularly shaped Pt NPs dispersed in IL and cellulose acetate lead to a nanocomposite that exhibits synergistic effects in the activity and durability enhancement of the catalyst . The authors have suggested that the presence of IL caused higher separation of the cellulose macromolecules which result in a higher flexible and lower viscous material. The ensuing nanocomposites displayed higher catalytic activity and stability when compared to the Pt NPs dispersed in the IL. Potential uses of cellulose/Pt nanocomposites in catalysis comprise the hydrogenation of cyclohexene  and hydrogen production .
Co NPs in cellulose matrices has been a topic of interest due to the potential application as magnetic nanocomposites. However, due to easy oxidation their use has been associated to the formation of metal alloys such as FeCo, as will be described in section 3.2.6. The properties of magnetic Co NPs are determined in large extent by surface atoms. In addition, crystallinity, size distribution, particles shape and neighboring particles, affect the response of the material when submitted to a magnetic field. Therefore the matrix in which the NPs are embedded, in this case cellulose, has strong influence on the magnetic properties of the NPs as well as the distance between them .
The structure and morphology of Co NPs synthesized in cellulose matrix and resulting magnetic properties have been reported . The authors have used two distinct chemical routes to investigate the effect on the structural properties of the NPs. In the borohydride reduction amorphous Co–B or Co oxide composites were obtained in which a detrimental effect on the magnetic properties was observed as compared to bulk Co. In contrast, using a NaH2PO2 reduction method, well-ordered ferromagnetic cobalt nanocrystals were obtained in which the magnetic properties of the samples resemble those of bulk cobalt.
3.2.6. Metal alloys
The properties of metallic systems can be significantly varied by blending the metal components into intermetallic compounds and alloys. The diversity of compositions, structures, and properties of metallic alloys not only can originate new properties but might also improve certain properties of the metal components due to synergistic effects . The association of metal alloys (typically bimetallic) to cellulose yields interesting materials with well-defined, controllable properties and structures on the nanometer scale coupled with easier processing capability of the matrix. A tubular FeCo bimetallic nanostructure was obtained by using a cellulose/cobalt hexacyanoferrate (Fe–CN–Co) composite material as precursor . The metal was then deposited onto a cellulose template via H2 gas-phase reduction that converted the precursor in FeCo bimetallic NPs. The FeCo NPs formed hollow tubular structures that mimic the original precursor composite morphology via a template-direct assisted method.
Lightweight porous magnetic aerogels made of nanofibrils of VC and BC have been compressed into a stiff magnetic nanopaper . The thick cellulose fibrils act as templates for the growth of discrete ferromagnetic cobalt ferrite NPs forming a dry, lightweight, porous and flexible magnetic aerogel with potential application in microfluidics devices and as electronic actuators. PdCu/BC nanocomposites showing high catalytic activity have been obtained, in which the PdCu NPs were homogeneously and densely precipitated at the surface . Although the cost of these materials need to be considered, these compositesare of potential interest in water remediation processes because the Pd Cu alloy is considered the best catalyst for the denitrification of polluted water.
3.3. Multifunctional cellulose/metal nanocomposites
The combination of cellulose with distinct metal NPs to design multifunctional nanocomposites is an interesting approach to extend the scope of these materials to several areas of applications. A fluorescent nanocomposite exhibiting antibacterial activity has been achieved through the functionalization of NFC with luminescent silver metal nanoclusters . A novel type of supramolecular native cellulose nanofiber/nanocluster adduct was obtained by using poly(methacrylic acid) (PMMA) as the mediator between Ag nanocluster and cellulose. The PMMA not only stabilized the Ag nanoclusters but also allowed hydrogen bonding between the particles and cellulose. Another example reports Au and Ag NPs as colorfast colorants in cellulose materials for textiles with antimicrobial and catalytic properties .
Also the combination of metal NPs with metal oxides is an emerging strategy to produce a range of multifunctional cellulose nanocomposites. The linkage of Ag NPs on magnetite containing BC substrates has been reported to produce magnetic and antimicrobial composites . The possibility of bringing together diverse types of inorganics NPs and distinct cellulose matrices opens a new field for future applications, where the design of natural based multifunctional materials will be privileged.
4. Concluding remarks and future trends
The combination of metal nanoparticles and distinct types of cellulose matrices takes benefit of the properties of both components and simultaneously might result in properties due to synergistic effects. Besides the nature of the components in the final nanocomposite, the performance of the final material depends on the preparative methodologies employed in their production. This review has shown the relevance on the nanocomposite performance not only of the type of metal NPs used as fillers but also the origin of the cellulose matrix. In this context, methods that allow the chemical modification of both components, metal NPs and cellulose matrices, appear a very promising field of research to develop new functional materials. The combination of diverse metal NPs in cellulosic matrices is an important but less exploited strategy to prepare multifunctional composites. Fundamental studies concerning physico-chemical interactions that occur between the composite components have been scarce despite their obvious relevance in the optimization of the materials properties. Finally, the impact of these nanocomposites on health and environment is an issue in the agenda of the scientific community but whose importance will increase due to the commercialization of products based on these materials.
|DP||Degree of polymerization|
|FFT||Fast Fourier transform|
|HRTEM||High resolution transmission electron microscopy|
|SEM||Scanning electron microscopy|
|SERS||Surface enhanced Raman scattering|
R.J.B. Pinto and M.C. Neves thank Fundação para a Ciência e Tecnologia (FCT) for the grants SFRH/BD/45364/2008 and SFRH/BPD/35046/2007, respectively. The authors acknowledge FCT (Pest-C/CTM/LA0011/2011), FSE and POPH for funding.
Sanchez C. Rozes L. Ribot F. Laberty-Robert C. Grosso D. Sassoye C. Boissiere C. Nicole L. 2010 Chimie douce: A land of opportunities for the designed construction of functional inorganic and hybrid organic-inorganic nanomaterials. 1 3 39
Manorama S. V. Basak P. Singh S. 2011 Anti-Microbial Polymer Nanocomposites.In Trindade T. & Daniel-da-Silva A. L. (Eds.) Singapura Pan Stanford Publishing 249 264
Belgacem M. N. Gandini A. 2008 Amesterdam: Elsevier
Goncalves G. Marques P. A. A. P. Pinto R. J. B. Trindade T. Pascoal Neto. C. 2009 Surface modification of cellulosic fibres for multi-purpose TiO(2) based nanocomposites. 69 7-8 1051 1056
Martins N. C. T. Freire C. S. R. Pinto R. J. B. Fernandes S. C. M. Neto C. P. Silvestre A. J. D. Causio J. Baldi G. Sadocco P. Trindade T. 2012Submitted.
Shen J. Song Z. Qian X. Ni Y. 2011 A Review on Use of Fillers in Cellulosic Paper for Functional Applications. 50 2 661 666
Kim J. Yun S. Ounaies Z. 2006 Discovery of cellulose as a smart material 39 12 4202 4206
Klemm D. Heublein B. Fink H. P. Bohn A. 2005 Cellulose: Fascinating biopolymer and sustainable raw material. 44 22 3358 3393
Roberts J. C. 1996 Glasgow: Blackieeditor.
Sjöström E. 1993 London Academic Press
Klemm D. Schumann D. Kramer F. Hessler N. Hornung M. Schmauder H. P. Marsch S. 2006 Nanocelluloses as innovative polymers in research and application.In Klemm D. (ed.) 205 49 96
Czaja W. Krystynowicz A. Bielecki S. Brown R. M. 2006 Microbial cellulose- the natural power to heal wounds. 27 2 145 151
Trovatti E. Serafim L. S. Freire C. S. R. Silvestre A. J. D. Neto C. P. 2011 Gluconacetobacter sacchari: An efficient bacterial cellulose cell-factory. 86 3 1417 1420
Iguchi M. Yamanaka S. Budhiono A. 2000 Bacterial cellulose- a masterpiece of nature’s arts. 35261 270
Klemm D. Schumann D. Udhardt U. Marsch S. 2001 Bacterial synthesized cellulose- artificial blood vessels for microsurgery. 26 9 1561 1603
Martins N. C. T. Freire C. Pinto R. J. B. Fernandes S. Pascoal Neto. C. Silvestre A. Causio J. Baldi G. Sadocco P. Trindade T. 2012 Electrostatic assembly of silver nanoparticles onto nanofibrillated cellulose for the development of antibacterial paper products. DOI: 10.1007/s10570-10012-19713-10575.
Klemm D. Kramer F. Moritz S. Lindstrom T. Ankerfors M. Gray D. Dorris A. 2011 Nanocelluloses: A New Family of Nature-Based Materials. 50 24 5438 5466
Belgacem M. N. Gandini A. 2011 Production, Chemistry and Properties of Cellulose-Based Materials.In Plackett D. (ed.) John Wiley & Sons, Ltd 151 178
Balazs A. C. Emrick T. Russell T. P. 2006 Nanoparticle polymer composites: Where two small worlds meet. 314 5802 1107 1110
Dankovich T. A. Gray D. G. 2011 Bactericidal Paper Impregnated with Silver Nanoparticles for Point-of-Use Water Treatment. 45 5 1992 1998
Wu D. Fang Y. 2003 The adsorption behavior of p-hydroxybenzoic acid on a silver-coated filter paper by surface enhanced Raman scattering. 265 2 234 238
Ma W. Fang Y. 2006 Experimental (SERS) and theoretical (DFT) studies on the adsorption of p-, m-, and o-nitroaniline on gold nanoparticles. 303 1 1 8
Ngo Y. H. Li D. Simon G. P. Gamier G. 2011 Paper surfaces functionalized by nanoparticles. 163 1 23 38
Jiang T. Liu L. Yao J. 2011 In situ Deposition of Silver Nanoparticles on the Cotton Fabrics. 12 5 620 625
El -Shishtawy R. M. Asiri A. M. Abdelwahed N. A. M. Al-Otaibi M. M. 2011 In situ production of silver nanoparticle on cotton fabric and its antimicrobial evaluation. 18 1 75 82
Montazer M. Alimohammadi F. Shamei A. Rahimi M. K. 2012 In situ synthesis of nano silver on cotton using Tollens’ reagent. 87 2 1706 1712
He J. H. Kunitake T. Nakao A. 2003 Facile in situ synthesis of noble metal nanoparticles in porous cellulose fibers. 15 23 4401 4406
Pinto R. J. B. Marques P. A. A. P. Pascoal Neto. C. Trindade T. Daina S. Sadocco P. 2009 Antibacterial activity of nanocomposites of silver and bacterial or vegetable cellulosic fibers. 5 6 2279 2289
Johnston J. H. Nilsson T. 2012 Nanogold and nanosilver composites with lignin-containing cellulose fibres. 47 3 1103 1112
Li Z. Friedrich A. Taubert A. 2008 Gold microcrystal synthesis via reduction of HAuCl4 by cellulose in the ionic liquid 1-butyl-3-methyl imidazolium chloride. 18 9 1008 1014
Vainio U. Pirkkalainen K. Kisko K. Goerigk G. Kotelnikova N. E. Serimaa R. 2007 Copper and copper oxide nanoparticles in a cellulose support studied using anomalous small-angle X-ray scattering. 42 1 93 101
Li Q. Yao G. Zeng X. Jing Z. Huo Z. Jin F. 2012 Facile and Green Production of Cu from CuO Using Cellulose under Hydrothermal Conditions. 51 7 3129 3136
Benaissi K. Johnson L. Walsh D. A. Thielemans W. 2010 Synthesis of platinum nanoparticles using cellulosic reducing agents. 12 2 220 222
Johnson L. Thielemans W. Walsh D. A. 2011 Synthesis of carbon-supported Pt nanoparticle electrocatalysts using nanocrystalline cellulose as reducing agent. 13 7 1686 1693
Tankhiwale R. Bajpai S. K. 2009 Graft copolymerization onto cellulose-based filter paper and its further development as silver nanoparticles loaded antibacterial food-packaging material. 69 2 164 168
Dong H. Hinestroza J. P. 2009 Metal Nanoparticles on Natural Cellulose Fibers: Electrostatic Assembly and In Situ Synthesis. 1 4 797 803
Marques P. A. A. P. Nogueira H. I. S. Pinto R. J. B. Neto C. P. Trindade T. 2008 Silver-bacterial cellulosic sponges as active SERS substrates. 39 4 439 443
Sharifi N. Tajabadi F. Taghavinia N. 2010 Nanostructured silver fibers: Facile synthesis based on natural cellulose and application to graphite composite electrode for oxygen reduction. 35 8 3258 3262
Pinto R. J. B. Marques P. A. A. P. Martins M. A. Neto C. P. Trindade T. 2007 Electrostatic assembly and growth of gold nanoparticles in cellulosic fibres. 312 2 506 512
Ishida T. Watanabe H. Bebeko T. Akita T. Haruta M. 2010 Aerobic oxidation of glucose over gold nanoparticles deposited on cellulose. 377 1-2 42 46
Mary G. Bajpai S. K. Chand N. 2009 Copper (II) Ions and Copper Nanoparticles-Loaded Chemically Modified Cotton Cellulose Fibers with Fair Antibacterial Properties. 113 2 757 766
Kotelnikova N. Vainio U. Pirkkatainen K. Serimaa R. 2007 Novel approaches to metallization of cellulose by reduction of cellulose-incorporated copper and nickel ions. 25474 79
Cai J. Kimura S. Wada M. Kuga S. 2009 Nanoporous Cellulose as Metal Nanoparticles Support. 10 1 87 94
He J. H. Kunitake T. Nakao A. 2004 Facile fabrication of composites of platinum nanoparticles and amorphous carbon films by catalyzed carbonization of cellulose fibers. 4 410 411
Pirkkalainen K. Leppanen K. Vainio U. Webb M. A. Elbra T. Kohout T. Nykanen A. Ruokolainen J. Kotelnikova N. Serimaa R. 2008 Nanocomposites of magnetic cobalt nanoparticles and cellulose. 49 3 333 342
Omrani A. A. Taghavinia N. 2012 Photo-induced growth of silver nanoparticles using UV sensitivity of cellulose fibers. 258 7 2373 2377
Son W. K. Youk J. H. Park W. H. 2006 Antimicrobial cellulose acetate nanofibers containing silver nanoparticles. 65 4 430 434
Cady N. C. Behnke J. L. Strickland A. D. 2011 Copper-Based Nanostructured Coatings on Natural Cellulose: Nanocomposites Exhibiting Rapid and Efficient Inhibition of a Multi-Drug Resistant Wound Pathogen, A. baumannii, and Mammalian Cell Biocompatibility In Vitro. 21 13 2506 2514
Li S. M. Jia N. Zhu J. F. Ma M. G. Xu F. Wang B. Sun R. C. 2011 Rapid microwave-assisted preparation and characterization of cellulose-silver nanocomposites. 83 2 422 429
Li S. M. Jia N. Ma M. G. Zhang Z. Liu Q. H. Sun R. C. 2011 Cellulose-silver nanocomposites: Microwave-assisted synthesis, characterization, their thermal stability, and antimicrobial property. 86 2 441 447
Silva A. R. Unali G. 2011 Controlled silver delivery by silver-cellulose nanocomposites prepared by a one-pot green synthesis assisted by microwaves. 22 31 315605
Boufi S. Ferraria A. M. Botelho doRego. A. M. Battaglini N. Herbst F. Vilar M. R. 2011 Surface functionalisation of cellulose with noble metals nanoparticles through a selective nucleation. 86 4 1586 1594
Yokota S. Kitaoka T. Opietnik M. Rosenau T. Wariishi H. 2008 Synthesis of Gold Nanoparticles for In Situ Conjugation with Structural Carbohydrates. 47 51 9866 9869
Gruber S. Taylor R. N. K. Scheel H. Greil P. Zollfrank C. 2011 Cellulose-biotemplated silica nanowires coated with a dense gold nanoparticle layer. 129 1-2 19 22
Yang G. Xie J. Deng Y. Bian Y. Hong F. 2012 Hydrothermal synthesis of bacterial cellulose/AgNPs composite: A "green" route for antibacterial application. 87 4 2482 2487
Yang G. Xie J. Hong F. Cao Z. Yang X. 2012 Antimicrobial activity of silver nanoparticle impregnated bacterial cellulose membrane: Effect of fermentation carbon sources of bacterial cellulose. 87 1 839 845
Maneerung T. Tokura S. Rujiravanit R. 2008 Impregnation of silver nanoparticles into bacterial cellulose for antimicrobial wound dressing. 72 1 43 51
de Santa Maria. L. C. Santos A. L. C. Oliveira P. C. Barud H. S. Messaddeq Y. Ribeiro S. J. L. 2009 Synthesis and characterization of silver nanoparticles impregnated into bacterial cellulose. 63 9-10 797 799
Barud H. S. Barrios C. Regiani T. Marques R. F. C. Verelst M. Dexpert-Ghys J. Messaddeq Y. Ribeiro S. J. L. 2008 Self-supported silver nanoparticles containing bacterial cellulose membranes. 28 4 515 518
Jung R. Kim Y. Kim H. S. Jin H. J. 2009 Antimicrobial Properties of Hydrated Cellulose Membranes With Silver Nanoparticles. 20 3 311 324
Zhang T. Wang W. Zhang D. Zhang X. Ma Y. Zhou Y. Qi L. 2010 Biotemplated Synthesis of Gold Nanoparticle-Bacteria Cellulose Nanofiber Nanocomposites and Their Application in Biosensing. 20 7 1152 1160
Wang W. Zhang T. J. Zhang D. W. Li H. Y. Ma Y. R. Qi L. M. Zhou Y. L. Zhang X. X. 2011 Amperometric hydrogen peroxide biosensor based on the immobilization of heme proteins on gold nanoparticles-bacteria cellulose nanofibers nanocomposite. 84 1 71 77
Wang W. Li H. Y. Zhang D. W. Jiang J. Cui Y. R. Qiu S. Zhou Y. L. Zhang X. X. 2010 Fabrication of Bienzymatic Glucose Biosensor Based on Novel Gold Nanoparticles-Bacteria Cellulose Nanofibers Nanocomposite. 22 21 2543 2550
Pinto R. J. B. Neves M. C. Pascoal Neto. C. Trindade T. 2012 Growth and chemical stability of copper nanostructures on cellulosic fibers ACSSubmitted.
Yang J. Sun D. Li J. Yang X. Yu J. Hao Q. Liu W. Liu J. Zou Z. Gu J. 2009 In situ deposition of platinum nanoparticles on bacterial cellulose membranes and evaluation of PEM fuel cell performance. 54 26 6300 6305
Olsson R. T. Samir M. A. S. A. Salazar-Alvarez G. Belova L. Strom V. Berglund L. A. Ikkala O. Nogues J. Gedde U. W. 2010 Making flexible magnetic aerogels and stiff magnetic nanopaper using cellulose nanofibrils as templates. 5 8 584 588
Ifuku S. Tsuji M. Morimoto M. Saimoto H. Yano H. 2009 Synthesis of Silver Nanoparticles Templated by TEMPO-Mediated Oxidized Bacterial Cellulose Nanofibers. 10 9 2714 2717
Diez I. Eronen P. Osterberg M. Linder M. B. Ikkala O. Ras R. H. A. 2011 Functionalization of Nanofibrillated Cellulose with Silver Nanoclusters: Fluorescence and Antibacterial Activity. 11 9 1185 1191
Dallas P. Sharma V. K. Zboril R. 2011 Silver polymeric nanocomposites as advanced antimicrobial agents: Classification, synthetic paths, applications, and perspectives. 166 1-2 119 135
Hubsch E. Ball V. Senger B. Decher G. Voegel J. C. Schaaf P. 2004 Controlling the growth regime of polyelectrolyte multilayer films: Changing from exponential to linear growth by adjusting the composition of polyelectrolyte mixtures. 20 5 1980 1985
Roberts J. C. 1996 Paper Chemistry. Glasgow Blackie
Ribitsch V. Stana-Kleinschek K. Jeler S. 1996 The influence of classical and enzymatic treatment on the surface charge of cellulose fibres. 274 4 388 394
Hyde K. Dong H. Hinestroza J. P. 2007 Effect of surface cationization on the conformal deposition of polyelectrolytes over cotton fibers. 14 6 615 623
Song J. Birbach N. L. Hinestroza J. P. 2012 Deposition of silver nanoparticles on cellulosic fibers via stabilization of carboxymethyl groups. 19 2 411 424
Chou W. L. Yu D. G. Yang M. C. 2005 The preparation and characterization of silver-loading cellulose acetate hollow fiber membrane for water treatment. 16 8 600 607
Abdel-Halim E. S. Al-Deyab S. S. 2011 Utilization of hydroxypropyl cellulose for green and efficient synthesis of silver nanoparticles. 86 4 1615 1622
Nadagouda M. N. Speth T. F. Varma R. S. 2011 Microwave-Assisted Green Synthesis of Silver Nanostructures. 44 7 469 478
Thomas V. Namdeo M. Mohan Y. M. Bajpai S. K. Bajpai M. 2008 Review on polymer, hydrogel and microgel metal nanocomposites: A facile nanotechnological approach. 45 1 107 119
Carlson C. Hussain S. M. Schrand A. M. Braydich-Stolle L. K. Hess K. L. Jones R. L. Schlager J. J. 2008 Unique Cellular Interaction of Silver Nanoparticles: Size-Dependent Generation of Reactive Oxygen Species. 112 43 13608 13619
Fernandez A. Picouet P. Lloret E. 2010 Cellulose-silver nanoparticle hybrid materials to control spoilage-related microflora in absorbent pads located in trays of fresh-cut melon. 142 1-2 222 228
Kim S. S. Park J. E. Lee J. 2011 Properties and Antimicrobial Efficacy of Cellulose Fiber Coated with Silver Nanoparticles and 3-Mercaptopropyltrimethoxysilane (3-MPTMS). 119 4 2261 2267
Niu Z. Fang Y. 2006 Surface-enhanced Raman scattering of single-walled carbon nanotubes on silver-coated and gold-coated filter paper. 303 1 224 228
Cabalin L. M. Laserna J. J. 1995 Fast spatially resolved surface-enhanced Raman spectrometry on a silver coated filter paper using charge-coupled device detection. 310 2 337 345
Liu Z. Li M. Turyanska L. Makarovsky O. Patane A. Wu W. Mann S. 2010 Self-Assembly of Electrically Conducting Biopolymer Thin Films by Cellulose Regeneration in Gold Nanoparticle Aqueous Dispersions. 22 8 2675 2680
Koga H. Tokunaga E. Hidaka M. Umemura Y. Saito T. Isogai A. Kitaoka T. 2010 Topochemical synthesis and catalysis of metal nanoparticles exposed on crystalline cellulose nanofibers. 46 45 8567 8569
An D. Ye A. Deng W. Zhang Q. Wang Y. 2012 Selective Conversion of Cellobiose and Cellulose into Gluconic Acid in Water in the Presence of Oxygen, Catalyzed by Polyoxometalate-Supported Gold Nanoparticles. 18 10 2938 2947
Tan X. Deng W. Liu M. Zhang Q. Wang Y. 2009 Carbon nanotube-supported gold nanoparticles as efficient catalysts for selective oxidation of cellobiose into gluconic acid in aqueous medium. 46 7179 81
Luckham R. E. Brennan J. D. 2010 Bioactive paper dipstick sensors for acetylcholinesterase inhibitors based on sol-gel/enzyme/gold nanoparticle composites. 135 8 2028 2035
Turyanska L. Makarovsky O. Patane A. Kozlova N. V. Liu Z. Li M. Mann S. 2012 High magnetic field quantum transport in Au nanoparticle-cellulose films. 23 4 045702
Gamarra D. Munuera G. Hungría A. B. Fernández-García M. Conesa J. C. Midgley P. A. Wang X. Q. Hanson J. C. Rodríguez J. A. Martínez-Arias A. 2007 Structure−Activity Relationship in Nanostructured Copper−Ceria-Based Preferential CO Oxidation Catalysts. 111 29 11026 11038
Guillot S. Chemelli A. Bhattacharyya S. Warmont F. Glatter O. 2009 Ordered Structures in Carboxymethylcellulose-Cationic Surfactants-Copper Ions Precipitated Phases: in Situ Formation of Copper Nanoparticles. 113 1 15 23
Gelesky M. A. Scheeren C. W. Foppa L. Pavan F. A. Dias S. L. P. Dupont J. 2009 Metal Nanoparticle/Ionic Liquid/Cellulose: New Catalytically Active Membrane Materials for Hydrogenation Reactions. 10 7 1888 1893
Himeshima N. Amao Y. 2003 Photoinduced hydrogen production from cellulose derivative with chlorophyll-a and platinum nanoparticles system. 17 6 1641 1644
Ferrando R. Jellinek J. Johnston R. L. 2008 Nanoalloys: From theory to applications of alloy clusters and nanoparticles. 108 3 845 910
Yamada M. Tsuji T. Miyake M. Miyazawa T. 2009 Fabrication of a tubular FeCo bimetallic nanostructure using a cellulose-cobalt hexacyanoferrate composite as a precursor. 12 1538 1540
Sun D. Yang J. Li J. Yu J. Xu X. Yang X. 2010 Novel Pd-Cu/bacterial cellulose nanofibers: Preparation and excellent performance in catalytic denitrification. 256 7 2241 2244
Sureshkumar M. Siswanto D. Y. Lee C. K. 2010 Magnetic antimicrobial nanocomposite based on bacterial cellulose and silver nanoparticles. 20 33 6948 6955